137 Cs Sorption Into Bentonite From Cidadap-Tasikmalaya As Buffer Material For Disposal Demonstration Plant Facility at Serpong - e-Repository BATAN
137 Cs sorption into bentonite from Cidadap-Tasikmalaya as buffer material for disposal demonstration plant facility at Serpong
View Table of Contents: Articles you may be interested in Appl. Phys. Lett. 90, 122114 (2007); 10.1063/1.2715477 J. Appl. Phys. 97, 043304 (2005); 10.1063/1.1844607 J. Chem. Phys. 120, 11144 (2004); 10.1063/1.1738638 J. Chem. Phys. 120, 7696 (2004); 10.1063/1.1688312 AIP Conf. Proc. 442, 485 (1998); 10.1063/1.56437
137 Cs Sorption Into Bentonite From Cidadap-Tasikmalaya
As Buffer Material
For Disposal Demonstration Plant Facility at Serpong
B. Setiawan , H. Sriwahyuni, NE. Ekaningrum, T. Sumantry
Radwaste Technology Center-National Nuclear Energy Agency,
PUSPIPTEK, Serpong-Tangerang, INDONESIA 15310
* Email: bravo @batan.go.id
Abstract. According to co-location principle, near surface disposal type the disposal demonstration plant facility will be build at
Serpong nuclear area. The facility also for anticipation of future needs to provide national facility for the servicing of radwaste
management of non-nuclear power plant activity in Serpong Nuclear Area. It is needs to study the material of buffer and backfill
for the safety of demonstration plant facility. A local bentonite rock from Cidadap-Tasikmalaya was used as the buffer materials.
Objective of experiment is to find out the specific data of sorption characteristic of Cidadap bentonite as buffer material in a
radwaste disposal system. Experiments were performed in batch method, where bentonite samples were contacted with CsCl
solution labeled with Cs-137 in 100 ml/g liquid:solid ratio. Initial Cs concentration was 10 M and to study the effects of ionic-8 -4
strength and Cs concentration in solution, 0.1 and 1.0 M NaCl also CsCl concentration ranging 10 – 10 M were added in
solution. As the indicator of Cs saturated in bentonite samples, Kd value was applied. Affected parameters in the experiment
were contact time, effects of ionic strength and concentration of CsCl. Results showed that sorption of Cs by bentonite reached
constantly after 16 days contacted, and Kd value was 10.600 ml/g. Effect of CsCl concentration on Kd value may decreased in
increased in CsCl concentration. Effect of ionic strength increased according to increased in concentration of background and
would effect to Kd value due to competition of Na ions and Cs in solution interacts with bentonite. By obtaining the bentonite
character data as buffer material, the results could be used as the basis for making of design and the basic of performanceassessment the near surface disposal facility in terms of isolation capacity of radwaste later.
Keywords: Demonstration plant, buffer, bentonite, sorption characterization PACS: 89.60.Ec
fabrication and radioisotope producer facilities at
Serpong. By taking into account the safety of people and environment, it is also intended to anticipate Radioactive Waste Technology Center located in future needs for preparation of facility for nationwide Serpong-Tangerang has main job to manage, conduct service of non-NPP radwaste management at Serpong research and service to all aspects related to area. According to International Atomic Energy radioactive waste management in Indonesia . By
Agency guidance, appropriated facility type for using evaporator, incinerator and compactor demonstration plant at Serpong is a near surface equipments, all radioactive wastes could be treated to disposal (NSD) type . So that all the technical produce radioactive waste packages in a 200L drum aspects related to the disposal type needs to be study and 350L or 950L concrete shell of containments. All and developed further. One of the technical aspects of waste packages and then storage in an interim that need to be developed is for buffer and backfill storage facilities, called as interim storage (IS) no 1 design concept of demonstration plant NSD type, and no 2 see Figure 1 .To anticipate decreasing of where specific information and data of buffer and
IS-1 and 2 capacity, then needed another facility to backfill materials must be obtained in order to accommodate the packages such as a radwaste created the design concept meet with condition of disposal facility which is also has a function as a demonstration facility purpose in Serpong. Several that purpose, a local bentonite has been planned as packages of existing waste at IS-1 and IS-2 could be buffer and backfill materials for planned disposal sent to the demonstration of radwaste disposal facility. facility. According to co-location principal, the demonstration plant of disposal to be used for low-activity radwaste with short half-life (less than 5 year)  from non- nuclear power plant activities is at same location with the waste producer such as reactor, nuclear element
4th International Conference on Mathematics and Natural Sciences (ICMNS 2012)
AIP Conf. Proc. 1589, 346-349 (2014); doi: 10.1063/1.4868816
© 2014 AIP Publishing LLC 978-0-7354-1221-7/$30.00
were initial and final activity of Cs-137 in solutions, and ܸ was the total volume of solution in 20 ml PE vial (ml), m was weight mass of samples
With ܽ denotes amount of metal ion absorped into solid phase per-mass unit and
ܾ is the amount of metal ion remains in solution per-volume unit.
(g), respectively. Radiocesium (Cs-137) used on the experiment relatively has long half-life (around 30 y) and has a similar behavior with K
- ion are mobile in a various environment system and easily assimilated with plants and organisms in water and soil so it can be easily enter into food chain in an enough wide range condition . In general, radionuclide ability to stay in environment depends on the magnitude of sorption capacity of solid phase as confinement material. And clay material such as bentonite is known has ability to absorb and isolate radionuclide  that is one of the reasons for the use of clay material as a barrier on a radwaste disposal facility system. Objective of the experiments are to study performance reliability in one of the disposal system that can ensure environment safety to people such as buffer material reliability through information of radiocesium sorption capacity of bentonite from Cidadap-Tasikmalaya, West Jawa. The results could be used for the basic of design concept preparation and performance assessment of NSD facility in term of radwaste isolation capacity and environment safety.
The used bentonite was obtained from a mining company PD Agribisnis dan Pertambangan Province of West Jawa, Karangnunggal-Tasikmalaya. Previously bentonite was clean up and then crushed, sieved to 100 mesh particle size and dried naturally before used as experiment samples. Radiocesium was obtained from Eckert & Ziegler and used without further preparation, while other chemical solutions were CsCl and NaCl from Merck. For radiometry analysis was used multichannel analyzer from Canberra.
Bentonite samples were contacted with a solution containing 10
M CsCl with solid:liquid ratio was ͳͲ
g/ml in a 20 ml PE vial. Contacting was conducted by using roller equippment and periodically sample was picked out. Solid and liquid phases was seperated by using syringe equipped with m filter. The aliquot and then measured their until reach the equilibrium contact time, and the saturated time was used for further experiments. For the effect of ionic strength experiment has been added 0.1 and 1.0 M NaCl in solution, while for the effect of CsCl concentration the solution was added with inial concentration of CsCl ranged from 10
ൌ ܽ ܾ or
FIGURE 1. View of waste packages in IS-1 building
Reliability of material for buffer purpose could be known from their capacity to hold groundwater flow in order to avoid direct contact between groundwater with waste packages or at least be able to delay travel time of groundwater reaches waste packages were stored in disposal facility . Moreover the buffer material must be able to absorb any possibility of radionuclide release from disposal facility into environment. And the distribution of radioactive contaminant will be isolated just around the disposal facility. The higher radionuclide sorption capacity by buffer material then better the function of material to isolate any radionuclide release to environment. Figure 2 is illustrated a kind of NSD type disposal.
FIGURE 2. An illustration of NSD type disposal
Reliability indicator of buffer material called as distribution coefficient, ܭ
ൌ ܽܿݐ݅ݒ݅ݐݕ ݊ ݏ݈݅݀ ݄ܽݏ݁
ܽܿݐ݅ݒ݅ݐݕ ݊ ݈݅ݍݑ݅݀ ݄ܽݏ݁
10 M CsCl. All the experiments were done at FIGURE 4. Effect of ionic strength to Cs-137 Chemistry laboratory of PTLR-BATAN in 2012 FY. sorption into bentonite
Results of the ionic strength effect in solution to
RESULTS AND DISCUSSIONS
radiocesium sorption into bentonite samples were showed in Figure 4. Increasing in concentration of The result of uptake profile of Cs-137 as sorption
NaCl as background salt in solution has resulted kinetic data of bentonite expressed by distribution decreased of Kd values of Cs-137. This is expected
coefficient versus contact time was showed in Figure due to competition between Na and Cs ions in the
3. Seen that the values reached constantly after ܭ
ௗ solution into bentonite samples occurred .
contact time of 16 days, with value around 10.600 ܭ
- 8 ml/g at CsCl concentration was 10 M.
Further experiment was to study the effect of CsCl concentration in solution when interacted with bentonite samples. The method was done by varying the initial concentration of CsCl in solution and then contacted to bentonite samples. Given initial
- 8 -4 concentrations were ranged from 10 to 10 M CsCl.
Contacting process was carried out for 16 days and the result was shown in Figure 5. In general seen that Kd values would decreased with increasing in CsCl concentration in the solution, and this is in accordance with the philosophy of the distribution coefficients of metal ions in the solid-liquid phase system.
FIGURE 3. Sorption kinetic of Cs-137 into bentonite
samples From the figure could be seen that sorption distribution of Cs-137 into bentonite samples has been occurred in 2 steps. This information corresponds to the information that bentonite is non- metallic mineral composed of 2 layers where the sorption process of metal ion on their interlayer through ion exchange processes .
FIGURE 5. effect of CsCl concentration to Cs-137
sorption into bentonite From the explanation shows that the Cs-137 sorption ability of bentonite from Cidadap-Tasikmalaya was good enough to absorb the Cs-137 occurred in solution, which was seen from the high values
ܭ ௗ obtained. The values of radiocesium into ܭ
bentonite samples have demonstrated the suitability of bentonite material when it will be used as a buffer material on the radwaste disposal system in the near future. The use of bentonite in the design of NSD is very helped to improve the disposal facility and also host rock ability to isolate radwaste did not release into environment.
A series of radiocesium sorption experiments into bentonite samples from Cidadap-Tasikmalaya have been done where sorption capacity of bentonite from Tasikmalaya have a pretty good results seen from
ܭ ௗ values reached around 10.600 ml/g after contacted in 16 days. Saturated of Cs-137 sorption into bentonite was achieved in 2 stages reflecting that bentonite was a double layer mineral. Increasing in the initial concentration of CsCl in solution has lowered the
values, and increasing in concentration of NaCl has decreased the values. There were expected due to ܭ
the limited capacity of bentonite samples and due to a
competition between Na and Cs ions interacted with active site of bentonite. The data were hopely to be used as one input for the safety assessment on a radwaste disposal activity in the near future.
1. PTLR, Strategic Plan of PTLR 2010-2014, PTLR-BATAN, 2010 – in Indonesian.
2. BATAN, Indonesia National Report for the
Simulated Joint Convention Group Session: on
the Safety of Spent Fuel and on the Safety of Radioactive Waste Management, Tokyo, ANSN- IAEA, 2010.
3. Y., Kawakami, Review of Site Evaluation
Activities for a RW Disposal Facility in Jawa Island, Report of IAEA EBP-Asia Expert
Mission, Serpong–Banten, Indonesia, 25-29 Feb 2008, Vienna, IAEA, 2008
4. D., Susilowati, “Preliminary Assessment on Conceptual Design of Near Surface Disposal for Radwaste”, Proc. Result of Researches and Activities of PTLR 2009 Year, PTLR-BATAN, 2010, pp.279-288 - in Indonesian
5. IAEA, Safety Guide, Siting of Near Surface
Disposal Facilities, SS no. 111-G-3.1, Vienna, IAEA, 1994.
6. S. Staunton and M. Roubaud, Clay and Clay Minerals, Vol. 45, No.2, pp.251-260 (1997).
7. RM., Cornell, J. Radioanal Nucl Chem 171, pp.483-500, (1993).
8. Encyclopedia of Geological Science, Mc Graw- Hill, NY (1978).
9. DM.,Di Toro, et.al., Env. Scie. Technol. 20, pp.55-61 (1986).